# Blending of Aggregate

date post

18-Jul-2016Category

## Documents

view

27download

3

Embed Size (px)

description

### Transcript of Blending of Aggregate

Aggregate Blending, Absorption & Specific Gravity 1

AGGREGATE BLENDING,

ABSORPTION, & SPECIFIC GRAVITY

Aggregate Blending, Absorption & Specific Gravity 2

Topics to be Covered Aggregate Specific GravitiesAggregate Specific Gravities

GradationsGradations

Blending StockpilesBlending Stockpiles

BatchingBatching

Combined Specific GravitiesCombined Specific Gravities

Aggregate Blending, Absorption & Specific Gravity 3

Specific Gravity Tests for Aggregates

Two tests are neededTwo tests are needed

Coarse aggregate (retained on the Coarse aggregate (retained on the 4.75 mm sieve)4.75 mm sieve)

Fine aggregate (passing the 4.75 mm Fine aggregate (passing the 4.75 mm sieve)sieve)

Aggregate Blending, Absorption & Specific Gravity 4

Gsa =

Mass of Aggregate,oven dry

Apparent Specific Gravity, Gsa

Volume of aggregate

Aggregate Blending, Absorption & Specific Gravity 5

Gsb =Mass of aggregate,

oven dry

Bulk Specific Gravity, Gsb

Vol of agg, + surface voids

Vol. of water-perm. voids

Surface Voids

Aggregate Blending, Absorption & Specific Gravity 6

Effective volume = volume of solid aggregate particle + volume of surface voids not filled with asphalt

Gse =

Effective Specific Gravity, Gse

Effective Volume

Absorbed asphalt

Vol. of water-perm. voidsnot filled with asphalt

Mass, drySurface Voids

Solid Agg.Particle

Aggregate Blending, Absorption & Specific Gravity 7

Water Absorption

SSD weight - Oven dry weight

Oven dry weight

Surface Voids

Solid Agg.Particle

Aggregate Blending, Absorption & Specific Gravity 8

Coarse Aggregate Specific Gravity

ASTM C127ASTM C127 Dry aggregateDry aggregate Soak in water for 24 hoursSoak in water for 24 hours Decant waterDecant water Use preUse pre--dampened towel to get SSD conditiondampened towel to get SSD condition Determine mass of SSD aggregate in airDetermine mass of SSD aggregate in air Determine mass of SSD aggregate in waterDetermine mass of SSD aggregate in water Dry to constant massDry to constant mass Determine oven dry massDetermine oven dry mass

Aggregate Blending, Absorption & Specific Gravity 9

Coarse Aggregate Specific Gravity

Aggregate Blending, Absorption & Specific Gravity 10

Coarse Aggregate Specific Gravity

Aggregate Blending, Absorption & Specific Gravity 11

Coarse Aggregate Specific Gravity Calculations

GGsbsb = A / (B = A / (B -- C)C) A = mass oven dryA = mass oven dry B = mass SSDB = mass SSD C = mass under waterC = mass under water

GGs,SSDs,SSD = B / (B = B / (B -- C)C) GGsasa = A / (A = A / (A -- C)C) Water absorption capacity, %Water absorption capacity, %

Absorption % = [(B Absorption % = [(B -- A) / A] * 100A) / A] * 100

Aggregate Blending, Absorption & Specific Gravity 12

Given:Given:Mass oven dry Mass oven dry -- 3625.5 (A)3625.5 (A)Mass SSD Mass SSD -- 3650.3 (B)3650.3 (B)Mass under Water Mass under Water -- 2293.0 (C)2293.0 (C)

Coarse Aggregate Specific Gravity Calculations - Example Problem

Aggregate Blending, Absorption & Specific Gravity 13

Apparent Specific Gravity Apparent Specific Gravity -- GGsasaA / (A A / (A -- C)C)

Bulk Specific Gravity Bulk Specific Gravity -- GGsbsbA / (B A / (B -- C)C)

Absorption, %Absorption, %(B (B -- A) / AA) / A

Coarse Aggregate Specific Gravity Calculations - Example Problem

Aggregate Blending, Absorption & Specific Gravity 14

Apparent Specific Gravity Apparent Specific Gravity -- GGsasa3625.5/ (3625.53625.5/ (3625.5--2293.0) = 2.7212293.0) = 2.721

Bulk Specific Gravity Bulk Specific Gravity -- GGsbsb3625.5 / (3650.3 3625.5 / (3650.3 -- 2293.0) = 2.6712293.0) = 2.671

Absorption, %Absorption, %(3650.3 (3650.3 -- 3625.5) / 2293.0 = 0.68 %3625.5) / 2293.0 = 0.68 %

Coarse Aggregate Specific Gravity Calculations - Example Problem

Aggregate Blending, Absorption & Specific Gravity 15

Fine Aggregate Specific Gravity ASTM C128ASTM C128

Dry aggregateDry aggregate Soak in water for 24 hoursSoak in water for 24 hours Spread out and dry to SSDSpread out and dry to SSD Add 500 g of SSD aggregate to pycnometer of known Add 500 g of SSD aggregate to pycnometer of known

volumevolume PrePre--filled with some waterfilled with some water

Add more water and agitate until air bubbles have been Add more water and agitate until air bubbles have been removedremoved

Fill to calibration line and determine the mass of the Fill to calibration line and determine the mass of the pycnometer, aggregate and waterpycnometer, aggregate and water

Empty aggregate into pan and dry to constant massEmpty aggregate into pan and dry to constant mass Determine oven dry massDetermine oven dry mass

Aggregate Blending, Absorption & Specific Gravity 16

Fine Aggregate Specific Gravity

Aggregate Blending, Absorption & Specific Gravity 17

Fine Aggregate Specific Gravity

Aggregate Blending, Absorption & Specific Gravity 18

Fine Aggregate

Specific Gravity

Aggregate Blending, Absorption & Specific Gravity 19

Fine Aggregate Specific GravityCalculations

GGsbsb = A / (B + S = A / (B + S -- C)C) A = mass oven dryA = mass oven dry B = mass of pycnometer filled with waterB = mass of pycnometer filled with water C = mass pycnometer, SSD aggregate and waterC = mass pycnometer, SSD aggregate and water S = mass SSD aggregateS = mass SSD aggregate

GGsb,SSDsb,SSD = S / (B + S = S / (B + S -- C)C) GGsasa = A / (B + A = A / (B + A -- C)C) Water absorption capacity, %Water absorption capacity, %

Absorption % = [(S Absorption % = [(S -- A) / A] * 100A) / A] * 100

Aggregate Blending, Absorption & Specific Gravity 20

Fine Aggregate Specific GravityCalculations - Example Problem

Given Given A = mass oven dry =489.3A = mass oven dry =489.3B = mass of pycnometer filled with water = 666.5 B = mass of pycnometer filled with water = 666.5 C = mass pycnometer, SSD aggregate and C = mass pycnometer, SSD aggregate and

water = 982.3water = 982.3S = mass SSD aggregate = 500.1S = mass SSD aggregate = 500.1

Aggregate Blending, Absorption & Specific Gravity 21

Fine Aggregate Specific GravityCalculations - Example Problem

GGsbsb = A / (B + S = A / (B + S -- C) = 498.9/(666.5+500.1C) = 498.9/(666.5+500.1--982.3)982.3)= 2.707= 2.707

GGsb,SSDsb,SSD = S / (B + S = S / (B + S -- C) = 500.1/(666.5+500.1C) = 500.1/(666.5+500.1--982.3)982.3)= 2.714= 2.714

GGsasa = A / (B + A = A / (B + A -- C) = 498.9/(666.5+498.9C) = 498.9/(666.5+498.9--982.3)982.3)= 2.725= 2.725

Water absorption = [(S Water absorption = [(S -- A) / A] * 100 = A) / A] * 100 = (500.1(500.1--498.9)/498.9 = 0.24 %498.9)/498.9 = 0.24 %

Aggregate Blending, Absorption & Specific Gravity 22

Aggregate Gradation

Distribution of particle sizes expressed Distribution of particle sizes expressed as percent of total weightas percent of total weight

Determined by sieve analysisDetermined by sieve analysis

Aggregate Blending, Absorption & Specific Gravity 23

Types Of Gradations* Open graded

- Few points of contact- Stone on Stone contact- High permeability

* Well graded- Good interlock- Low permeability

* Gap graded- Lacks intermediate sizes- Good interlock- Low permeability

Aggregate Blending, Absorption & Specific Gravity 24

100

0.075 .3 2.36 4.75 9.5 12.5 19.0

Percent Passing

control points

max density line

maxsize

nommaxsize

Sieve Size (mm) Raised to 0.45 Power

Design Aggregate Structure

Superpave Aggregate Gradation

Aggregate Blending, Absorption & Specific Gravity 25

Definitions Nominal Maximum Nominal Maximum Aggregate SizeAggregate Size

one size larger than the first sieve to one size larger than the first sieve to retain more than 10%retain more than 10%

MaximumMaximum Aggregate SizeAggregate Size one size larger than nominal maximum one size larger than nominal maximum

sizesize

1001009072654836221594

100998972654836221594

Aggregate Blending, Absorption & Specific Gravity 26

Superpave Mix Size Designations

Superpave Nom Max Size Max SizeDesignation (mm) (mm)

19.0 mm 19 25

12.5 mm 12.5 19

9.5 mm 9.5 12.5

Aggregate Blending, Absorption & Specific Gravity 27

19.0 mm

9.5 mm

12.5 mm

Aggregate Blending, Absorption & Specific Gravity 28

Blending of Aggregates

Reasons for blendingReasons for blendingObtain desirable gradationObtain desirable gradationSingle natural or quarried material not Single natural or quarried material not

enoughenoughEconomical to combine natural and Economical to combine natural and

process materialsprocess materials

Aggregate Blending, Absorption & Specific Gravity 29

Blending of Aggregates

Numerical methodNumerical methodTrial and errorTrial and errorBasic formulaBasic formula

Aggregate Blending, Absorption & Specific Gravity 30

Blending of Aggregates

P = P = AaAa + Bb + Cc + + Bb + Cc + .. Where:Where:

P = P = % of material passing a given sieve for % of material passing a given sieve for the blended aggregates the blended aggregates

A, B, C, A, B, C